Mechanism of Antibacterial Activity via Morphology Change...
Embed Size (px)
Transcript of Mechanism of Antibacterial Activity via Morphology Change...
Mechanism of Antibacterial Activity via Morphology Change of α‑AgVO3: Theoretical and Experimental Insights Regiane Cristina de Oliveira,*,† Camila Cristina de Foggi,‡ Mayara Mondego Teixeira,†
Maya Dayana Penha da Silva,† Marcelo Assis,† Eric Mark Francisco,†
Bruna Natalia Alves da Silva Pimentel,‡ Paula Fabiana dos Santos Pereira,† Carlos Eduardo Vergani,‡
Ana Lućia Machado,‡ Juan Andres,§ Lourdes Gracia,§,∥ and Elson Longo†
†CDMF-UFSCar, Universidade Federal de Saõ Carlos, P.O. Box 676, 13565-905 Saõ Carlos, SP Brazil ‡FOAr-UNESP, Universidade Estadual Paulista, P.O. Box 1680, 14801903 Araraquara, SP Brazil §Departament de Química Física i Analítica, Universitat Jaume I, 12071, Castello ́ de la Plana, Spain ∥Department of Physical Chemistry, University of Valencia, 46100, Burjassot, Spain
*S Supporting Information
ABSTRACT: The electronic configuration, morphology, optical features, and antibacterial activity of metastable α-AgVO3 crystals have been discussed by a conciliation and association of the results acquired by experimental procedures and first-principles calcu- lations. The α-AgVO3 powders were synthesized using a coprecipitation method at 10, 20, and 30 °C. By using a Wulff construction for all relevant low-index surfaces [(100), (010), (001), (110), (011), (101), and (111)], the fine-tuning of the desired morphologies can be achieved by controlling the values of the surface energies, thereby lending a microscopic understanding to the experimental results. The as-synthesized α-AgVO3 crystals display a high antibacterial activity against methicillin-resistant Staphylococcus aureus. The results obtained from the experimental and theoretical techniques allow us to propose a mechanism for understanding the relationship between the morphological changes and antimicrobial performance of α-AgVO3.
KEYWORDS: α-AgVO3, morphologies, first-principles calculations, photoluminescence, Wulff construction, antibacterial activity
AgVO3 is the most commonly occurring structure of silver vanadium oxide-based materials in the solid state.1 Four polymorphs, the metastable α-, γ-, and δ-forms and the more stable β-type, have been described.2,3 Fleury and Kohlmuller4
presented X-ray diffraction (XRD) results without structural analysis. Thenceforth, structural chemistry studies of these phases were developed.2,3,5−7 β-AgVO3 is the more stable polymorph and presents a monoclinic space group (I2/m No. 12),6 while α-AgVO3 is a metastable phase of the monoclinic C2/c (No. 15) system. α-AgVO3 is irreversibly transformed to β-AgVO3 at 200 °C.
2 Consequently, polymorphism is a property inherent to AgVO3. Metastable compounds offer tremendous opportunities to
obtain new materials with unusual properties that drive the efforts to understand and optimize their synthesis and stabilization. From the viewpoint of flourishing scientific interest and technological applications, the study of AgVO3 polymorphic materials provides an exciting platform for investigation owing to their versatile properties resulting from the diverse phase transitions of AgVO3. Our research group is
involved in a project devoted to studying complex metal oxides, such as α-Ag2WO4, as efficient microbial agents.
8 In addition, the synthesis and characterization of metastable phases such as β-Ag2WO4
9,10 and γ-Ag2WO4 11,12 and, in a very recent paper,
the synthesis and characterization of the stable phase of β- AgVO3
13 have also been reported. Working closely with experimentalists on the comprehension of the surface proper- ties of complex multifunctional materials requires the use and development of several computational strategies where a precise knowledge of their optimal geometry and structure is a mandatory prerequisite to computational modeling. The- oretical simulations can address several properties of the materials: the morphology, the surface structure below genuine thermodynamic environments, and analytical descriptors of antibacterial activity. With the information provided by the theoretical results, a plethora of experimental data can be better matched to computer simulations, providing synergy between
Received: January 18, 2017 Accepted: March 14, 2017 Published: March 14, 2017
© 2017 American Chemical Society 11472 DOI: 10.1021/acsami.7b00920 ACS Appl. Mater. Interfaces 2017, 9, 11472−11481
07 , 2
different experimental techniques and theory. This work is a continuation of these earlier studies, in which a combination of theory and experiments is performed, and our motivation is principally fueled by discovering a novel synthesis of metastable phases with novel properties. Previous works on the synthesis of metastable α-AgVO3 have
either reported the requirements of high temperatures or long reaction times or showed poor crystalline structures or low purity.2,14,15 Later, Shao and co-workers16 successfully synthe- sized pure α-AgVO3 with a high crystallinity through a biomimetic process. Very recently, McNulty et al.17 described the achievement of α-AgVO3 nanowires via a hydrothermal treatment and the structural transformation of α-AgVO3 to the tunnel-structured β-AgVO3 by annealing at 475 °C. Here, we synthesized α-AgVO3 samples by using the
coprecipitation (CP) method at low temperatures. The characterizations of the structures, morphologies, and optical properties were performed by experimental techniques such as X-ray diffraction (XRD) with Rietveld analysis, Raman (MR) spectroscopy, field-emission scanning electron microscopy (FE- SEM), ultraviolet−visible (UV−vis) diffuse reflectance spec- troscopy, and photoluminescence (PL). Later, we focus on the analysis of the antibacterial activity against methicillin-resistant Staphylococcus aureus (MRSA), by determining the minimum inhibitory/bactericidal concentrations (MIC/MBC). First- principles quantum-mechanical density functional theory (DFT) calculations are used to supplement these experimental techniques.
2. EXPERIMENTAL PROCEDURES 2.1. Synthesis. The α-AgVO3 were acquired by CP method. For
this are used silver nitrate (AgNO3, 99% purity, Synth) and ammonium monovanadate (NH4VO3, 99% purity, Sigma-Aldrich). Initially, 1 mmol of NH4VO3 and 1 mmol of AgNO3 were individually melted in 35 mL of water, under agitation, at 30 °C. The solutions were jumbled, and a quick materialization of solid α-AgVO3 (yellow coloration) occurred. The CP was performed at 10, 20, and 30 °C. The powders was washed with distilled water and dried in an oven at 60 °C for 12 h. 2.2. Characterization. The α-AgVO3 powders were characterized
by X-ray diffraction using a Rigaku-DMax/2500PC with Cu Kα radiation (λ = 1.5406 Å) in the 2θ range from 10° to 80° with a scanning speed of 0.02°/min. The Rietveld refinements were done by using the general structure analysis (GSAS) program using with XDR patterns in the 2θ range from 10° to 110° with a scanning rate of 0.01°/min. Raman spectroscopy was done in a spectrometer (Horiba Jobin-Yvon) coupled to a CCD Synapse detector and an argon ion laser, operating at 532 nm with maximum power of 1.2 mW. The spectra were measured in the range from 5 to 1000 cm−1. UV−vis spectra were collected with a Varian spectrophotometer model Cary 5G in diffuse reflection mode. The morphologies were investigated by field emission scanning electron microscopy (FE-SEM) with a Supra 35-VP Carl Zeiss instrument operated at 15 kV. In addition, transmission electron microscopy (TEM) analyses operating at 200 kV and energy dispersive X-ray spectroscopy (EDS) were performed with a FEI microscope model Tecnai G2 F20. The PL measurements were performed with a Monospec 27 monochromator (Thermal Jarrel Ash) coupled to a R446 photomultiplier (Hamamatsu Photonics). A krypton ion laser (Coherent Innova 90 K) (λ = 350 nm) was used as excitation source, keeping its maximum output power at 500 mW. All experiments measurements were performed at room temperature. 2.3. Theoretical Methods. First-principles total-energy calcu-
lations were performed using the DFT framework as implemented in the VASP package.18 The generalized gradient approximation in the Perdew−Burke−Ernzerhof formulation for electron exchange and correlation contributions to the total energy were used to solve the
Kohn−Sham equations.19,20 The relaxed systems were generated by means of the conjugated gradient energy minimization scheme when the Hellmann−Feynman forces converged to less than 0.01 eV/Å per atom. Projector augmented wave pseudopotentials were used to describe the electron−ion interaction. A cutoff energy of 520 eV was selected to truncate the plane-wave expansion, and the Brillouin zones have been sampled through Monkhorst−Pack special k-points grids that ensure geometrical and energetic convergence for the α-AgVO3 structures. Vibrational frequency calculations were performed at the Γ- point, and the dynamical matrix was computed by numerical evaluation of the first derivative of the analytical atomic gradients.
Stoichiometric slabs for low Miller index surfaces of monoclinic α- AgVO3 structure were modeled, a